PREFERRED KNOTS FOR USE IN CANYONS
PREFERRED KNOTS FOR USE IN CANYONS
Bushwalkers Wilderness Rescue Squad 1 PREFERRED KNOTS FOR USE IN CANYONS David Drohan Abstract On behalf of the Bushwalker’s Wilderness Rescue Squad (BWRS) Rock Squad, the author is conducting a series of tests in a voluntary capacity to determine the preferred knots that could be used in recreational canyoning. This paper will be of interest to all abseilers who have to retrieve their ropes. The project is planned for three stages. Stage one is now complete and this paper focuses on the tensile strength and slippage of various knots. Cyclic loading and rope pull down issues have also been investigated.
139 hours of actual testing has been conducted to date. This time does not include the considerable time to plan, analyse and write up the report. This paper was presented at the Outdoor Recreation Industry Council NSW conference in Sept 2001.
For further information regarding BWRS visit the web site at http://www.bwrs.org.au Introduction Recreational canyoning groups are questioning the traditional knots to join tape or rope. It has been argued that the traditional Double Fisherman’s Knot (Figure 1-a) to join ropes is very tight to undo after use and often catches on obstacles during rope pull down. The Tape Knot (Figure 1-b) can be difficult to adjust and now some groups have started using unconventional knots such as the Overhand Knot for joining rope or tape (Figure 1-c & d). There is also evidence that some groups have been using smaller than usual size tape or cord for anchors, in order to reduce cost.
This is done on the pretext that their group will only use the anchor sling once and they believe it is strong enough. It is commonly regarded that 50mm flat tape or 25mm tube tape is acceptable for use in anchor slings. The project will explore if smaller size slings could be used, such as flat 25mm or maybe even 19mm polyester tape. The proposal for this project was outlined in March 2000. This paper discusses tests conducted to determine various knot strengths, slippage and ease of rope pull down for various rope/tape materials.
Literature Review Existing Information on Ropes, Aging and Knot Strength/Slippage The author has researched published information on the strength and slippage of knots in rope and webbing. There is significant data on the rated strength of new tape and rope as indicated in
Bushwalkers Wilderness Rescue Squad 2 the sample of catalogues and specifications (see references). However only a couple of references have been sighted that provide data on strength of knots tied in Kernmantle rope. Warild (1990 p33&34) provides information on recommended and non-recommended knots showing the static strength and falls taken for each knot.
He states “the performance of most knots is variable and depends on many factors, rope diameter, wet or dry, knot packing and to a lesser extent temperature” (p33). He suggests the bulky knots appear to have a clear advantage especially in 8 or 9 mm rope and the Overhand Loop (knot) performs inconsistently. Whilst Warilds’ tables are very helpful, the current author has not been able to access the test data on which they were based, and there are no test results for knot slippage. Luebben (1996, p7) also provides some data on the strength of knots, but no supporting references are provided.
Long (1993, p54), mentions that the Water (Tape) knot should be checked frequently, as it has the tendency to come untied.
Much testing has been conducted by the international organisation of alpine clubs, Union Internationale des Association d’Alpinisme, (UIAA) on falling climbers and the equipment that breaks their fall. It is important to understand what causes the severity of the fall and so understand what is called a fall factor. Benk & Bram (Edelrid) describe the fall factor (FF) as the proportion of fall and the length of rope run out. The fall factor describes the severity of the fall and determines the load on the entire system. The most serious fall a climber could take in normal circumstances is FF2, that is the length of free fall (say 20m) divided by the length of rope paid out being (say 10 m) therefore 20/10 = 2.
This means 10m of rope must absorb the fall energy of a 20 m free fall. Abseilers do not take such extreme shock loads on their equipment. Warild (1990 p 15) argues that the worst fall factor a caver (abseiler) could take if one of the two anchor bolts snapped would only be FF0.6. The probability of a FF0.6 fall is extremely low and the most abseilers should ever expect for a well rigged rope is FF0.3. Warild states the most convincing evidence that caving (static) ropes are strong enough is the complete lack of accidents due to ropes failing under shock loads from caving (or abseiling in canyons).
Warild (1990, p 17) mentions ropes could be damaged by mechanical deterioration by 10 FF0.1 minor shock loads, caused by prusiking or rough abseiling and suggests this is an avenue for investigation. One of the future tests in Stage 2 will explore this issue, as old ropes (that are too stiff to abseil on) are often used as back up anchor ropes.
Polyamide static ropes used for canyoning can be old. There is no “use by date” based only on age. The Blue Water Technical Manual (2001) provides information on when to retire your static rope, such as damage from sharp edges, glazing from fast abseils or soft hollow or lumpy sections in the rope. Replacement is based on wear and tear. Age is not mentioned as a limiting criteria. What has been observed for ropes over 10 years old is that they often become too stiff to handle and abseil on. This is due to the mantle shrinking and so becomes less pliable. Blue Water recommends the shelf life for one of their unused dynamic ropes as five years.
Blue Water admits there is no conclusive evidence from nylon manufacturers regarding aging of unused ropes. Warild argues on p 17 that age does affect used ropes and gives data for a 4.5 year old 9mm BWII rope that indicates it can only withstand four FF1 falls, where a new rope can take 41 such shocks. AS4142.3 (1993) requires new 11mm static ropes used for rescue to withstand two FF2 falls. Provided the abseiler does not intentionally shock load the rope the way a climber could, age is not an issue, as polyamide static ropes can withstand some shock loading. Even with the worst normal abseiling shock load of FF0.6 the old rope should survive one such shock load, as Warilds tests indicated the 4.5 year old rope could withstand four of the higher FF1 falls.
It appears aging affects a ropes ability to survive shock. The five-year rule only apples to dynamic ropes as they are designed for high shock loads. Static ropes are not required to be condemned when they reach five years old as they are not intended to take high shock loads.
Bushwalkers Wilderness Rescue Squad 3 Many rope manufacturers treat their rope with a “dry treatment”. This involves coating the nylon fibres of the rope with either silicon or teflon. Details on the process are difficult to obtain from manufacturers. This process is done so the rope will absorb less water when wet and therefore maintain its strength. Warild (1990, p16) discusses that water absorption in nylon rope makes it less abrasion resistant and reducing its static and shock strength by up to 30%. Some of the Edelrid ropes tested in this study were “dry” treated. For natural laid fibre rope Marks Engineering Handbook (1987, p88) states that the shorter the bend in standing rope, the weaker the knot (based on Millers experiments 1900).
However it appears to be a different story for nylon ropes. A report (the author wishes to remain anonymous), discovered that knots in Kernmantle (polyamide) rope failed at the point of maximum compression due to the knot compressing one strand of the rope sufficiently that the heat generated by friction caused the strand to become plastic and then fail. Petzl (2000) (an outdoor gear manufacturer) provides some information on alternative knots on their web page technical manual, such as recommending the Abnormal Figure 8 Knot to join two abseil ropes together. There is no supporting data for this recommendation.
There is also useful data at this web site for UIAA limits and design criteria, such as that harnesses should not be loaded to more than 15kN.
Delaney (2000) from the Australian School of Mountaineering states he is not aware of any testing of aged tape and rope as typically found in canyons and suggests there is only limited information on knot slippage, but he could not provide any supporting test data. Manufacturer’s Rated Strength The rated strength given by the product manufacturer is the minimum strength that the material will fail at, normally given in kilonewtons (kN). Most of the older equipment was rated in kilograms force (kg).
To convert to kg, multiply by 1000 (newtons) then divide by 10 (gravity rounded up). For example; a karabiner is marked as 22kN.
22kN x 1000 = 22000(N) /10 = 2200 kg. A quick simple rule is just multiply kN by 100 to get kg. Adequate testing of the product has been conducted by the manufacturer to determine the mean breaking strength. Therefore the minimum or “rated” breaking strength can be determined. US and European companies that have extensive production undertake comprehensive testing of large samples from many batches. Therefore an accurate statistical figure can be determined. Some products like karabiners have a “Sigma 3” rating which is three standard deviations back from the mean. However many overseas companies only use two standard deviations back from the mean for rope and tape products.
To explain standard deviations (std dev), Freund (1988 p76) defines for the results that create a normal (bell shaped) distribution as follows: About 68% of the values will lie within one standard deviation of the mean, hence about 16% are outside the 1 std dev on the low side. About 95% of the values will lie within two standard deviation of the mean, hence only about 2.5% are outside the 2 std devs on the low side. 99.7% values will lie within three standard deviation of the mean, hence only about 0.15% are outside the 3 std devs on the low side.
Some Aust/NZ rope/tape manufacturers do not use statistical calculations to determine their rated strength for the materials used in this study.
Toomer (2000) has clarified that the rated
Bushwalkers Wilderness Rescue Squad 4 strength used by Australian rope manufactures is based on a number of batch tests, using the lowest breaking specimen. Usually the rated strength is rounded down to the nearest 100 kg. Small (2000) from Donaghys Industries (a New Zealand webbing manufacturer) stated the webbing (WPM25-OPG63 &WPM50-OA900) tested in this project is uncertified. The only testing conducted by the company on these products were by random sample and the “rated” load stated in the specification sheet is based on the minimum strength from the random testing. The random sample is based on three specimens from the end of a batch run.
Batches were only tested when the company had altered a part of the manufacturing process or for some other reason. No statistical methods are employed to determine the minimum break load for random sample tests.
Working Load Limit The working load limit (WLL), sometimes referred to as the safe working load, is the maximum static load that should be applied to a rated piece of equipment. Dividing the rated strength by the Safety Factor (SF) will give the WLL for that piece of equipment. Our example of a karabiner rated at 2200kg divided by SF5 for hardware will give a 440kg WLL. Understanding Safety Factors Most rope and hardware manufacturers give their product a rated strength. To determine the WLL a Safety Factor (SF) is used. Jensen (1974) describes safety factor as the ratio of ultimate stress (rated strength) to allowable stress (WLL).
The safety factor is based on a number of considerations including risk to human life, wear and tear of the product, aging and the type of loading that may be encountered. To understand how SFs are determined, he gives examples ranging from 2 to 10 depending on the machine and application. Engineers have agreed that 5 is acceptable for lifting loads involving humans. SF5 has been adopted as the SF used for abseiling equipment hardware. Bateman & Toomer’s (1990) Australian Lightweight Vertical Rescue Instructors (ALVRI) verbal advice during the course as recorded by the author, discuss that SF5 is acceptable for hardware, however rope and tape must include a factor to account for loss of strength due to the knot.
ALVRI use a strength loss of one-third (33%) for any knot used in rescue. That is 0.67 strength remaining in the rope. The original rope strength with no knot is divided by the strength remaining due to knot of 0.67. This gives a ratio of 1.49. Multiplying the SF5 by this ratio of 1.43 will give a figure of 7.46. This figure has been rounded up to give SF8. Based on this rationale, AS 4142.3 (1993), notes the SF as not less than 8 is considered appropriate. It is noted that the American Blue Water (2000) catalogue use the US Fire department’s SF15.
An appropriate SF is important. An excessive SF may add a significant weight or volume penalty to the equipment you have to carry if you wish to maintain the existing WLLs.
A SF that is too low may lead to equipment failure with possible loss of life. What else needs to be done? From the literature review it is clear there is still a lot to learn about knot strength and slippage in rope and tape. The tests conducted in this study provide further data on these issues however are not exhaustive. Such a study would require access to research databases covering strength of rope materials to determine the extent of research already conducted on this subject and how best to build on this knowledge.
Project Design This project aimed to determine the best possible knot for joining ropes and slings together in a canyon. A useful side benefit was to identify any hazards evident in alternative knots. A process
Bushwalkers Wilderness Rescue Squad 5 of elimination determined the preferred knots. The knots being considered were eliminated in a step by step process based on the results from tests of A to E (listed below). The preferred knot (for each application) is the one that has the best results and has not been disregarded due to a safety issue. The first stage of the process examined the static forces involved.
The definition of “static” in this case, is load not subjected to dynamic forces. Objectives: Stage One A. To determine the tensile strength and slippage of standard knots in slings. B. To determine the tensile strength and slippage of alternative knots that could be used to join tape and rope.
C. To determine the tensile strength of certain single strand ropes without knots. D. To determine if knots used to join slings or ropes slip under normal (cyclic) loading. E. To determine the ease of double rope pull down using various rope joining knots. Section A is used as a baseline for the strength of standard knots. Section B compares the strength of the alternative knots to Section A. Section C attempted to confirm the strength of the rope/tape used in Sections A and B, without the influence of the knot on rope strength. Any knots that were found unsafe after completion of Sections A to C were deleted from the remainder of the tests.
Sections D and E are the final set of tests to examine the preferred knots for canyon use.
A further two stages of the project are planned to consider the shock forces and aging process. More information on these topics is provided under “Further Research” latter in this paper. Method Testing Requirements In order to maintain repeatability, reliability and validity of the tests the author has referred to appropriate Australian standards. No standard could be found that gave a procedure for tensile testing of endless loops, therefore the author has adopted the philosophy of AS 4143.1(1993) for endless loop tests and has described the procedures followed in a later section of this paper.
For single strand rope testing AS 4143.1 (1993) is directly applicable and requires a gauge length of one metre (the distance between bollards) at the required pre-tensioned load. This indicates a test bed with a stroke of two to three metres would be required. Toomer (2000) from Spelean (an Australian rope manufacturer) indicated that the one metre length is important in order to have enough material between the gauge lengths when compared with the material wrapped around the bollards. The machines that the author had access to only had a maximum stroke of one metre. In an attempt to solve this problem the author noted that in AS 2001.2.3 (1988) which is one of the standards for testing seat belts, the procedure only required a gauge length of 200mm.
For this reason single strand tests using a gauge length of only 200mm were attempted. There are no standards for conducting the cyclic and rope pull down tests in this project. Again the author has described the procedures followed in a later section of this paper. Clem (2000) (former chairman of the Life Safety Section of the Cordage Institute, USA) provided useful advice on the testing requirements for tensile and dynamic testing of knots. His findings indicate apart from obvious criteria such as rope material and diameter, that more subjective issues can come into play. These include which side the tail comes out of the knot.
ie if the knot is tied right or left hand. The author has noted these concerns and attempts have been
Bushwalkers Wilderness Rescue Squad 6 made to record any unusual events during the tests by video recording a number of the tests and taking individual notes on test records. Clem advises the absolute minimum size of the sample would be six specimens of the same material. It is acknowledged that the sample should be larger, however due to resource constraints the author has chosen six specimens per sample based on Clem’s advice. Although a sample of six is less than ideal, AS 4143.1 (1993) only requires a report based on two successful test specimens. Therefore the authors sample is three times greater than the relevant standard requires.
Units used. The metric system of measurement has been used for this study. Length measurements: millimetres (mm) are used for measurement up to one metre and metres (m) for measurements greater than one metre. Force measurement: kilonewtons (kN) have been used for the tensile tests. For the cyclic and rope pull down tests kilograms (kg) were used. As manufacturers rate their equipment in kN it was decided the tensile tests would remain in that unit. Although Force (Newtons) equals mass (kg) times gravity, it was decided for the other tests that simulated the weight of people and arm strength required to pull ropes down, it would be simpler to express the results of measurements as kg mass units.
The Tests of stage One A. Tensile Strength and Slippage of Standard Knots in Slings A tensile test machine was used to test the rated strength of new tape and old rope made up into an endless sling by a knot. The slings were tested to failure. The joining knots were the Tape Knot for tape and the Double Fisherman’s Knot for rope.
B. Tensile Strength and slippage of Alternative Knots in Slings A tensile test machine was used to test the rated strength of alternative knots in tape and rope made up into endless slings. C. Single Strand Tensile Strength Single strand of rope is the terminology used by rope manufacturers to describe a single length of rope, it is not a single fibre of rope. The testing conducted in A & B was for endless slings, the rating given in the manufacturer’s specification was doubled as a consequence. The doubled rating was compared to the second standard deviation back from the mean breaking strength from each sample.
This is not ideal due to statistical differences in the size of the two samples being compared. To produce accurate values of strength loss due to a knot from the knot tests conducted in A& B, additional tests were conducted without a knot for the same material. This would make it possible to compare the results to determine a true strength loss due to a knot. Single strand tests are required for this. It is also reasonable to compare the breaking strength of the aged material without a knot to the rated strength to determine the strength loss due to age of the material.
D. Knot Slippage caused by Cyclic Loading Knot slippage under cyclic loading may be a more serious problem than slipping under a constant load. Repeated predetermined loads were placed on the tape or rope slings. The knots were measured for any slippage after each load application. E. Canyon Rope Pull Down In canyon abseils a double rope is slung around the anchor point and one end is pulled down to retrieve the rope after use. Tests were conducted to measure the force to pull a knot joining two ropes over various edges.
Bushwalkers Wilderness Rescue Squad 7 Knots Selected for Testing There are many knots capable of tying rope or tape together.
A knot used in a canyon environment must be safe. Safety in this context can be broken down into four sub headings. 3 & 4 are considered safety issues due to the extra time to correct problems. 1. Acceptable strength and slippage 2. Easy to check 3. Easy to tie and untie 4. Suitable for the intended application. That is, the knot won’t catch on an edge during pull down. These criteria were used to select the knots. The following knots may meet the criteria. The project plan aimed to determine which knots met all of the above criteria.
(a) Double Fisherman’s Knot in rope (b) Tape Knot in tape (c ) Overhand Knot in rope (d) Overhand Knot in tape (e) Rethreaded Figure Eight Knot (f) Abnormal Figure Eight Knot (g) Alpine Butterfly Knot (to tie ropes together) Figure 1
Bushwalkers Wilderness Rescue Squad 8 Where applicable the knots were tied right-handed. There is an exception for one of the Overhand Knot pull down tests that also included a left-handed knot. The Single Fisherman’s and Bowline to join ropes together were considered inappropriate due to known slippage issues. The Rethreaded Overhand knot (a Tape Knot for rope) did not have any obvious advantage over a Double Fisherman’s and so was not considered.
Obviously dangerous knots such as the Reef Knot or various slip knots were dismissed.
Other knots such as the Reef Knot backed up with a Double Fisherman’s Knot and also the Double Fisherman’s Knot to tie tape were eliminated before the testing began. The Reef backed up with a double fisherman’s has been used by some groups to overcome the issue of the Double Fisherman’s Knot being too tight to undo after use. It is considered this knot is too complicated and would be even more difficult due to its size to pull over a hard edge in rope pull down tests. The author has heard of parties tying anchor tape with a Double fisherman’s knot. It is assumed they consider this knot “fool proof” regarding slippage, however this knot uses a large amount of tape to tie and most canyoners do not distrust the Tape Knot enough to use this alternative knot.
Therefore the author has decided not to test this knot.
Materials, Knot Packing, Preparation & Conditioning Materials defined as new were purchased for the testing and were unused at the time of testing. Due to difficulties in accessing retailers purchase records, no attempt was made to determine the time lapse between actual manufacture date and purchase date. The actual manufacture date was not printed on the tape reels. Dates of known ropes/tape of known age are based on the purchase date. Old rope is considered acceptable to use in these tests as this rope is sometimes used as canyon slings and always used as abseil ropes. A new rope can only be used new once! Variables were kept to a minimum to improve repeatability such as: - Knowing the brand and age of the rope.
- Ensuring the 6 specimens per test are cut from the same piece of rope. - Checking that any core or mantle damage is within the ALVRI guidelines. Testing of some Sisal rope has been conducted, as canyoners may use this rope as slings in rarely visited canyons. This is done on environmental grounds, as it is believed sisal rope will rot and break down faster than nylon rope/tape when left in a canyon.
The material to be tested was formed into a sling (endless loop) by a joining knot. Figure 2 details the naming convention of the knot. The “Tails” are the rope/tape knot tail ends and the “Tension” is the section of rope/tape that form the sling. Figure 2 Knot Definitions
Bushwalkers Wilderness Rescue Squad 9 All knots in tape and rope were packed according to ALVRI guidelines. The guidelines recommend there shall be no cross overs in any part of the lay of the knot and the knot shall be pulled hand tight on each protruding section out of the knot to remove any rope slackness in the knot.
The tails should be long enough to tie a thumb knot. When these procedures are followed, the knot should look neat in appearance and should not have any unnecessary slippage occurring under normal load.
Although the length of a sling does not influence the load at which it will break, the author considered it would still be useful to standardise sling length. This was achieved by the use of a bollard jig for each machine. Due to the physical dimensions of each machine a standard size sling was not possible for this stage of the project. The CIT machine sling length was 380 ±15mm. The ADFA machine sling length was 255 ±15mm. Conditioning of dry samples to AS 4143.1 (1993) requires a standard atmosphere of 20 ±2 o C and a relative humidity of 65 ±2%. Whilst not all testing was conducted in an air conditioned facility, the temperature and relative humidity were monitored and testing was postponed if the relative humidity rose above 70% or the air temperature was less than 15 or greater than 30o C Conditioning for the tensile test wet samples was in water between 14 and 17o C, for a duration of between 45 to 60 minutes which is considered appropriate to simulate a rope in a waterfall whilst people are abseiling.
For the tensile tests refer to Annex B Sheet 2 to determine which wet samples were dry treated.
For the cyclic tests the rope/tape samples were not “dry” treated. Wet test specimens were tied into slings whilst dry, then placed into a bucket of cold water for approximately 10 minutes before the test. As each set of tests took 3 hours to conduct, cold water was poured onto the 6th and 10th cycle to prevent drying out. Dry tests were only conducted when the relative humidity was less then 67%, due to humidity possibly affecting the results by moisture tightening the knot and thus reducing slippage.
Equipment Tensile Testing Machines Two tensile testing machines were used to conduct the tensile tests.
One is located at the Mechanical Test Laboratory; Bruce Canberra Institute of Technology (CIT) (ACT). The other is at the Civil Engineering Test Laboratory - Australian Defence Force Academy (ADFA) (ACT). Bruce CIT The machine at Bruce CIT (Figure 3-a&b) is a Shimadzu universal tensile testing machine, rated to 25 tonne and is currently certified by the National Association of Testing Authorities (NATA) as a Class A machine for all loads in range. This machine can produce load elongation graphs, unfortunately they can not be scaled and are only to be used as a guide. On this machine the gauge length was measured between the cross heads on the machine.
The author worked in collaboration with the technical officer responsible for the operation of the machine. The CIT laboratory is maintained to the necessary temperature and humidity requirements.
Bushwalkers Wilderness Rescue Squad 10 (a) The CIT tensile testing machine cross heads (b) Dial controls (The rope is to hold the pipe bollards in place when the specimen breaks) Figure 3 Unfortunately the stroke of this machine was only 300mm. Due to the elongation of the material the machine often required a reset before the material broke (in some cases 2 or 3 times). This practice involved the hydraulic rams being reset whilst attempting the keep the cross heads in the current position. The specimen was unloaded about 10 to 20% for each reset. Fortunately nearly all specimens could have the elongation measured at 3.67kN before a reset was required.
The author has been reassured this practice does not affect the accuracy of the final breaking load, however it did affect the measurement of elongation at failure. The reset issue was the primary reason why access to another tensile machine was sought.
ADFA The machine at ADFA was used to conduct the remainder of the tensile tests that could not be conducted using the Bruce CIT machine. This machine (Figure 4-a) is an Autograph tensile testing machine, rated to 10 tonne with a stroke of 950mm. It can be fitted with special bollards that are designed to minimise bollard stress concentration. For sling tests the 65mm outside diameter bollards (Figure 4-b) (which are free to rotate) have a 10mm machined radius to cradle the rope. The gauge length was measured between the bollard centres. For single strand tests the 65mm outside diameter fixed bollards (Figure 4-c) have a 10mm machined radius spiral into the bollard to cradle the rope for the required three wrap turns.
This machine can produce scaled load elongation graphs. The machine has been certified by NATA as a Class A machine for all loads in range. Although not currently certified, the author has witnessed that the machine has been verified to within an accuracy of 100N to the requirements of the NATA certificate. The ADFA Lab is air-conditioned, but a roller door (located 20m away) to the outside was often open, which may have affected humidity.
(a) The ADFA Tensile Testing Machine (b) Sling bollard (c ) Single strand bollard Figure 4
Bushwalkers Wilderness Rescue Squad 11 Knot Cyclic Testing Rig A rig has been built to simulate the cyclic loads that occur when a rope is abseiled on, several times. The rig was set up to measure any slippage in knots caused by this type of cyclic loading. A sling tied with the knot to be tested was suspended from an overhead structure.(Figure 5-a) Each knot was marked so any slippage in the tail or out of the sling could be measured. Measurements were taken in the unloaded condition.
Either 50 or 100kg of weight were hung from the sling. Any slippage was measured when the sling was loaded (Figure 5-b). The sling was then unloaded using appropriate mechanical advantage, and was shaken for five seconds to simulate possible knot loosening by wind or handling by an abseiler. The sling was then reloaded and another set of measurements taken. This process was repeated 15 times. The Figure of 15 was considered appropriate for a maximum number of people likely to be abseiling the pitch.
(a) (b) (a) The cyclic testing rig showing the sling, the weight and the rope mechanical advantage for lifting the weight. (b) Sling tape showing the slippage marks on the “Tension” side. Figure 5 Rope Pull Down Friction Measurement Rig Any one who has been canyoning will know how varied the required force to pull down abseil ropes can be. Force can range from one hand for a 5m drop through to three people hanging off the rope under a waterfall to slowly move it down past 50m of friction points. Due to all the possible variables it was decided one standard cliff site would be used. Trial tests at Wee Jasper indicated a 15m cliff was acceptable to provide the required friction within the spring balance range.
Two sets of tests were planned using a natural and an artificial 90o hard edge for both dry and wet conditions. The first waterfall on Bungonia creek was selected as a good site to conduct the tests. The 9mm static ropes used in this series of tests had no dry treatment applied. Permission was gained from the Bungonia NPWS ranger to conduct a BWRS Rock Squad testing day held at the first waterfall in Bungonia Creek. The cliff edge consisting of volcanic quartz has two points of contact for the rope with the edges at 25o and 20o off vertical. The anchor sling was angled at 40o above horizontal.
The natural edge does not have a problem with excessive friction. As can be seen from Figure 6-a, a V shape groove could catch certain knots. There was a ledge 12.5m from the top edge to take load measurements from. Two knot pull down tests were conducted, one on the natural cliff edge and for the second a Bessa block was used for the hard edge tests. Unfortunately the Bessa block could not be
Bushwalkers Wilderness Rescue Squad 12 secured sufficiently to prevent movement, therefore the hard edge tests were invalid. Lack of time prevented the wet tests from being conducted. (a) The Bungonia cliff detailing the knot going (b) Profile of the Bungonia cliff edge. over the 25o edge Figure 6 In order to complete valid hard edge tests, the authors garage roof (Figure 7-a) was selected. The roof is 2.7m high and 2x4m lengths of 9mm static ropes tied together with the knot to be tested were used. A concrete Bessa block was secured so it would not move under rope loads. A second block was used to position the anchor pivot point.
The tests were standardised by using the block in the same position for all tests. A Spring balance has been used to measure the force required to start moving the knot over a 90o reverse edge and going over the 90o obtuse edge.
Significant friction within the measurement range of the spring balance was obtained without the need to simulate the weight of hanging rope. Trial tests determined that the 1.5kg weights (to simulate 25m of free hanging rope) on each rope end were not required due to the 45kg spring balance exceeding its limit. (a) The author using a spring balance to measure the load (b) The profile of the edges used for when pulling a knot over a 90 0 edge at his garage. the garage Figure 7 The rate of travel used in this series of tests was determined to be approximately 2 seconds per metre of rope pulled, ie 0.5m/s.
This rate of travel was considered appropriate in order to read
Bushwalkers Wilderness Rescue Squad 13 the spring scales. In actual canyon rope pull down situations the rate of travel of a person pulling down the ropes may be twice the speed for small pitches. There was evidence that fast rope pull downs sometimes required less load to pass over the edge. Unfortunately trial tests determined it was not possible to measure the load on the spring balance in the fast rope pull down tests, therefore the results obtained may be conservative. The hard edge (Figure 7-b) is considered one of the harshest edges that could be encountered so it is a good edge to test the knots being examined.
For the wet tests a garden hose was used to continually spray water over the Bessa block.
Loads & Test Weights In simulating the loads that could be applied in canyoning, the load of two people abseiling at once on a double rope (twin person or assisted abseiling) is used, as this load is the heaviest load that should be applied in the recreational activity of canyoning. ALVRI use a standard weight of 100kg for one person. Therefore the load of 200kg (1.96kN) is used to simulate two people on the abseil rope. The 200kg weight should be the WLL of ropes and tape used for canyon abseiling.
AS 4142.3 (1993) states 3.67kN (375kg) is the WLL for a rescue rope. Collecting strength and slippage data at this load will be of use to the rescue community.
Slippage measurements have been recorded when the tensile test machine reached a load of 1.96kN and 3.67kN. A final set of records have been taken when the test specimens failed. Load verses elongation graphs have been produced by the tensile test machines. For the Cyclic Loading tests, the aim was to determine if greater slippage at the knot would occur by the repeated application of a lighter load when compared to a standard 200 kg load applied only once. A load of 50kg representing a teenager and a load of 100kg representing an adult has been used in this series of tests. The cyclic loading test weights are made up of a cluster of calibrated 10kg and 20kg weights provided by Bruce CIT.
Test Apparatus and Measurement Equipment The tensile test machines were pretensioned, as required by AS4143.1 (1993). For each 9mm rope and tape specimen pretensioning was set at 0.1kN. For 11mm rope specimens the setting was 0.15kN. With the specimen pretensioned between the bollards of the tensile test machine, the gauge mark length was measured with a tape measure. This was the zero load measurement. The gauge length is defined as a mark on each bollard structure to which measurements were taken to determine sling elongation. Elongation measurements were taken at zero load, 1.96 kN (200 kg), 3.6 kN (375 kg) and failure.
The tensile test machines crosshead rate of travel was set at 40mm per minute. All tensile tests had the knot positioned mid away on the sling between the bollards. Refer to Figure 4-a, photograph of the ADFA machine that shows a typical sling set up. Vernier callipers were used to measure knot slippage. The specimens were marked at the four protrusions from the knot with a suitable contrasting coloured pen (that would not affect the strength of the material). The tail lengths were measured at zero load, as it was expected the tails would shorten and the marks would move within the knot. Tail lengths were then measured at each predetermined load.
The mean “Tail” slippage could then be calculated. The “Tension” slippage data provided is the summation of the two measurements taken between the mark and the knot. Measurements were taken at each predetermined load by stopping the tensile testing machine long enough to record the dimensions. Care was taken to place the vernier callipers on
Bushwalkers Wilderness Rescue Squad 14 the same section of the test specimens for all the readings. Accuracy is believed to be within ±1 mm. A spirit level, adjustable protractor and a 30m tape measure were carried into the Bungonia waterfall site to survey the cliff edge (Figure 6b). A Bessa block was carried in (and out) for the hard edge tests. Two spring balance scales rated to either 25kg or 45kg were available for the rope pull down tests. If loads were higher than 25kg then the 45kg scale was used. The load on the scale was noted as the knot moved each time. Reading accuracy was assessed to be within ±1kg using this method.
The 25kg spring balance was calibrated using test weights of 5kg 10kg & 20kg and was found to be accurate. The 45kg spring balance was calibrated using test weights of 5kg, 10kg, 20kg, 30kg & 40kg and found to require a correction for accuracy. A correcting factor has been applied to the results of the 45kg spring balance readings.
Results Refer to the Annexes A to E for tables and graphs of the results of this study. Annex C is not used as this series of tests was not successful. Discussion The knot strength losses quoted in this report are for percentage strength loss due to a knot compared to the rope strength. Manufacturers tend to provide rated strength as percentage remaining in the material. Annexes A&B also tabulate the strength data as percentage strength remaining in the rope for reference only. Statistical data is given for strength data to determine the lowest breaking strength based on 2 standard deviations (std devs) back from the mean.
2 std dev was chosen as the sample was too small for 3 std devs to give a meaningful number. Additional most overseas manufacturers use 2 std devs for their ratings.
The ramifications of relatively small samples and the approach to comparisons means there is some statistical uncertainty. It is therefore not possible to state the values for knot strength in absolute terms. However, the strength data provided can be used as a general guide. Slippage data discussed in the paper is at the abseil working load of 1.96kN. The slippage data provided in Annex A & B is given at the loads of 1.96kN (200kg), 3.67kN (375kg) and failure. The slippage data is a guide only. Standard deviation calculations were completed for these measurements but have not been reported.
There was significant scatter from the mean (up to 30%) and it is believed the sample would have to be much greater to provide conclusive statements about rope/tape slippage.
The slippage data presented in Annex A & B for the1.96 and 3,67kN loads could not be obtained for some materials when using the CIT machine. This was due to the large cross heads obstructing access to the specimens. Refer to Figure 3 (a) for a photograph of the cross heads. The remaining factor of safety of the material is determined relative to a 1.96kN (200kg) load. Dividing the knot’s 2 std dev breaking strength back from the mean by the 1.96kN load derives this safety factor. The equation for this is SF=(Mean breaking load –2 std devs)/Abseil WLL
Bushwalkers Wilderness Rescue Squad 15 For this case the breaking load includes the weakness of the knot.
Therefore an additional knot factor is not included in this safety factor. As a result of this logic, the safety factor for any material should always be greater than 5. (SF5 is for loads involving humans) Results Analysis Knot Age & Material Sling Breaking Strength 2 Std Dev back from Mean (kN) Mean "Tail" slippage at 1.96 kN (mm) Total "Tension" slippage at 1.96 kN (mm) Loss of Strength due to knot Tape Tape New 50mm flat tape New 25mm tube tape 24.64 21.52 Not recorded Not recorded Not recorded Not recorded 52% 42% Double Fisherman’s 1 year old 11mm static rope 36.43 5 48 42% Rethreaded Figure 8 1 year old 11mm static rope 30.11 1 45 52% Overhand new 50 mm flat tape 17.94 25 Not recorded 65% Overhand 1 year old 11mm static rope 22.05 12 51 65% Abnormal Fig 8 15 year old 11mm static rope 24.10 16 203 62% Alpine Butterfly 1 year old 11mm static rope 29.97 14 54 52% Table 1 Summary of Strength Loss due to Knot & Slippage For detailed information refer to Annex A & B Table 1 provides an abridged summary of the strength loss due to knot & slippage data that is provided in Annex A and Annex B.
The following discussion refers to these Annexes, this table is provided for quick reference.
A. Tensile Strength & Slippage of Standard Knots in Slings Double Fisherman’s Knot (Figure 1-a) (refer to sheet A-2) One year old Blue Water 11mm rope had a strength loss due to the knot of 42%. The 18 year old Blue Water 11mm rope had a strength loss of 70%. The difference between the 1 and 18 year old rope tied with the same knot is 28%. It appears the aging of the old rope may account for a ≅30% strength loss. Graph A-4 is typical of the slope of elongation verses load which was generally non-linear. For new 10mm & 12mm Sisal rope the strength loss due to the knot was 36% & 9 %. The 9% may be explained, if the manufacturer’s rated strength included a knot.
It could also be explained if the manufacturers rated strength for the rope was 3 standard deviations below the mean rope breaking strength. Then a sample of rope well above the rated strength would give the low apparent strength reduction.
Graph A-5 is typical of the slope of elongation verses load which was very jagged due to the rope fibres in the knot beginning to fail, as well as minor slippage in the knot. New 7mm & 9mm Riviory rope gave unexpected results of 2% & 6 % strength loss due to the knot. The abseil working load “Tension” slippage averaged out at 49mm for both 9mm and 11mm rope. The “Tail” creep was 6mm at this load. The sisal rope slipped less than the kermantle rope. Its “Tension” slippage was only 30mm due to the laid strands locking and thus reducing slippage.
The remaining SF for 10mm Sisal rope was only 4.
All other materials tested had SFs in excess of 5
Bushwalkers Wilderness Rescue Squad 16 Tape Knot (Figure 1-b) (refer to sheet A-1) These results indicate new Polyester flat tape (19 & 50mm) had a strength loss due to the knot of around 50%. The 25mm flat had the greatest strength loss due to knot of 58%. New Polyamide 25mm tube tape, had a strength loss due to of the knot of 42%. Graph A-3 is typical of the slope of elongation verses load which was generally linear until failure, however their were noticeable dips in the graphs believed to be due to slippage in the knot as it became tight.
Slippage data was not recorded for most of this series of tests.
However, the cyclic tests on tape do provide further data on slippage. The remaining SF when using 19mm or 25mm slings tied with a tape knot is only 3. The remaining SF for 50mm flat and 25mm tube was good at 13 and 11. B Tensile Strength & Slippage of Alternative Knots Overhand Knot for rope (Figure 1-c) (refer to Annex B sheet B-1) One year old Blue Water 11mm rope had a strength loss due to the knot of 65%. Graph B-4 is typical of the slope elongation verses load which was generally exponential until failure. At near failure it was noted one specimen displayed a partial roll back in the knot.
(Similar to the abnormal Figure 8 Knot) This was an unusual event and should be examined with further testing.
The strength loss due to knot for the six year old 9mm rope was high at 75%. It is unclear whether rope age is affecting the results here. The remaining SF when using a 1.96kN load was acceptable at 5. The remaining Factor of Safety for one year old Blue Water II 11mm rope was good at 11. There was only a 5% difference in strength or slippage between the wet and dry tests for the 6 year old Edelrid 9mm static rope. The Edelrid “dry” treatment is likely to have protected the rope from moisture and so loss of strength.
The abseil working limit “Tension” slippage averaged 65mm for both the 9mm and 11mm rope.
“Tail” slippage was 10mm. The Overhand Knot had acceptable standard deviation figures for strength. This goes against Warild’s (1990) observations that reported the strength of this knot as being inconsistent. For new 12mm Sisal rope the strength loss due to the knot was low at 41 %. Graph B-5 is typical of the slope of elongation verses load, which was jagged as the rope fibres began to fail, as well as minor knot slippage.
Of the Overhand Knot samples tested on the tensile testing machines, the majority appeared to fail at the point of maximum compression inside the knot. The knots geometry uses a chocking effect for gripping the two ropes which may be the reason why it is not as strong as the other knots tested. The chocking action may concentrate all the load onto a small area thus causing a compression point which leads to failure. The Double Fisherman’s Knot, which also failed at the point of maximum compression just inside the knot, was not affected by a chocking action but rather a gripping action over a greater proportion of the knot.
Hence the Double Fisherman’s Knot is stronger than the Overhand Knot.
Bushwalkers Wilderness Rescue Squad 17 Overhand Knot for tape (Figure 1-d) (refer to sheet B-1) For new Polyester flat tape (25mm & 50mm), the strength loss due to the Overhand Knot was between 61 to 65%. The remaining SF when using a 1.96kN load for the 25mm flat and 25mm tube tape was only 3. For the wet and dry 50mm flat samples, the remaining SF was between 9 and 10. There was no major difference in strength or slippage between wet and dry tests for 25 or 50mm flat polyester tape. The result for the three-year-old Polyamide 25mm tube tape, which had a strength loss due to the knot of 82%, was alarming.
Mean breaking strength was only 7.16kN and the standard deviation of the sample tested was very small at 0.42 (indicating very repeatable results). If the material were new, it is estimated the breaking strength would be 12.6kN. The results give a breakage 56% less then what was expected. It seems unlikely the ageing effect would be this bad for tape that was only bought in June 97. The sample had been used as a club hand line during that time and had been stored appropriately when not in use. Although the sample tape was dirty (It was washed and dried before testing) no serious abrasion was detected apart from some minor fluffing.
Graph B-3 is typical of the slope of elongation verses load which was generally linear until failure. Rethreaded Figure Eight Knot (Figure 1-e) (refer to Annex B sheet B-2) One year old BW 11mm rope had a strength loss due to the knot of 52%. The new 7mm and 9mm Rivory rope had a low strength loss due to the knot of 24% and 30% respectively. The remaining SF with the 1.96kN load for the 9mm and 11mm ropes were excellent at 13 and 15 respectfully and acceptable for the 7mm cord at 8. The abseil working limit “Tension” slippage averaged at 44mm. Average “Tail” slippage was only 1mm. This knot had the least slippage (especially tail) when compared to the other knots of the same material.
Abnormal Figure Eight Knot (Figure 1-f) (refer to Annex B sheet B-2) Breaking strength was similar averaged at 14.8kN between the two Edelrid wet and dry samples. This was probably due to the “dry” treatment on this rope. Strength loss due to knot was between 62% to 64%, however this rope was aged. The breaking strength of the older Blue water 9mm rope sample was a lot stronger at 24.1kN compared to the two Edelrid samples that were not as old. All 9mm rope specimens tested had at least one roll back, four rolled back twice and one specimen rolled back three times. The lowest first roll back occurred at 2.1kN ( the weight of two abseilers) Graph B-6 is typical of the slope on the graph of elongation verses load, which was dramatic, as the knot displayed either partial or complete roll-backs.
Significant “Tension” slippage was already occurring at the abseil-working load, with an average “Tension” slippage of 165mm. “Tail” slippage was only an average of 10mm. Average “Tension” slippage at failure for the 3 sets of tests conducted was 410mm. On one specimen the “Tail” had slid in 120mm to the point where the tail was flush with the knot before it broke. Another specimen had a “Tension” slippage of 633mm at failure. No significant slippage difference was noted between wet and dry samples.
Another example of how dangerous this knot can be is to tie the knot with inappropriate tail lengths and have the knot poorly packed. In this configuration, it is possible for two people